UNIVERSIDAD DE VALLADOLID
ESCUELA DE INGENIERIAS INDUSTRIALES
Grado en Ingeniería Mecánica
Pre-consolidation of hybrid textiles for the
production of web based thermoplastic
García Pelayo, Miguel
RIB: Sánchez Bascones, Ma
TFG REALIZADO EN PROGRAMA DE INTERCAMBIO
Pre-consolidation of hybrid textiles for the production of web based
Miguel García Pelayo
15 septiembre 2017
El objetivo de este TFG es desarrollar un nuevo proceso de pre-consolidación del
material no tejido que se usará posteriormente para crear una pieza de fibra de carbono
reciclada. El proceso de pre-consolidación nuevo permite una forma más efectiva de
calentar, presionar y enfriar. Para ello se ha diseñado un prototipo con una máquina de
aire caliente y una prensa de rodillos.
PALABRAS CLAVE QUE DEFINEN EL TFG:
The work was submitted to the
Institut für Textiltechnik Augsburg gGmbH
Univ.-Prof. Dr.-Ing. Stefan Schlichter
Pre-consolidation of hybrid textiles for the production of web based
Miguel Garcia Pelayo
examiner: Univ.-Prof. Dr.-Ing. Stefan Schlichter
examiner: Prof. Dr. Siegfried R. Horn
Dr.-Ing. Philipp Abel
Pre-consolidation of hybrid textiles for the
production of web based thermoplastic
Recycling carbon fiber is an up to date theme around the world. The institute of textile tech-nology of Augsburg has developed a process to use carbon fibers and plastic fibers to create a nonwoven material which is then pre-consolidated into a preform and finally used to build a part. The aim of this thesis is, to develop a new pre-consolidation process of the hybrid textile that permit a more effective way of heating, pressing and cooling.
Preliminary trials have been done in order to obtain some technical data. Then the design process has been elaborated starting with a definition of the functional structure, which is divided in sub-functions. Six Concepts have been created, compared and evaluated.
The Concept selected is composed of a hot air machine that allows a fast and homogenous heating, a rolling press, a conveyer belt to ensure an accurate transport of the preform and a roll which permit to store and transport the preform easily.
Table of Contents
2.3.2 Preparation to the Dilo compact fabric conditioning ... 23
2.4 Instruments of development methodology ... 24
3 Preliminary trials ... 28
3.1 Abstract ... 28
3.2 Introduction and objectives ... 28
3.3 Trials heating with the DEMA Hand-press TP1400 ... 29
3.4 Trials heating up with infrared oven ... 31
3.4.1 Cooling and pressing with metal weight applying contact pressure ... 32
3.4.2 Cooling and pressing with metal applying pressure with the DEMA Hand-press TP1400 ... 34
3.4.3 Cooling and pressing with metal applying contact pressure in a reduced area . 36 3.5 Trials heating up with induction plates ... 40
3.6 Trials heating with hot air ... 41
4 Theoretical design ... 43
4.1 Request list... 43
4.2 Functional Structure ... 44
4.2.1 Building the overall function ... 45
4.2.2 Dividing the overall function into sub-functions ... 45
4.2.3 Complete functional structure ... 47
4.3 Definition of the concepts ... 48
4.5 Vulnerability Analysis ... 55
5 Development of the concept ... 59
5.1 The heating process ... 59
5.2 The Cooling and pressing process ... 63
5.3 The transport process ... 66
5.4 The rolling up process ... 67
5.5 Total production and energy consumption ... 68
6 Summary and Outlook ... 69
Bibliography ... 71
7 Appendix ... 74
List of Figures
Fig. 1.1: Schematic vision of the overall process. The main theme of this thesis is
highlighted in bold ... 13
Fig. 2.1: Schematic of PAN and pitch based carbon fiber manufacturing process. [Ash13] ... 16
Fig. 2.2: Structure of the carbon crystals. [Ehr06] ... 16
Fig. 2.3: Graphic of composite demand and waste in kilotons per year. [Mel16] ... 20
Fig. 2.4: Side view of the Dilo machine used by the ITA. [Mar17] ... 23
Fig. 2.5: General procedure for developing and designing. [PBF07]... 25
Fig. 2.6: Overall function divided into sub-functions. [Fel13c] ... 26
Fig. 2.7: Vulnerability analysis through a value profile. [Fel13d] ... 27
Fig. 3.1: Infrared oven. [EnM16] ... 31
Fig. 3.2: Hybrid textile before being heated and pressed (left) and preform after being heated and pressed (right). ... 32
Fig. 3.3: Two layers heated together in the oven 20 seconds (left) and 30 seconds (right). ... 34
Fig. 3.4: Final thickness of trials P1, P2 and P3. ... 36
Fig. 3.5: Final thickness with the hand-press at 90ºC. ... 36
Fig. 3.6: Schematic draw of each way of applying pressure used. ... 37
Fig. 3.7: Schematic view of the final thickness of the preform measured ... 37
Fig. 3.8: Final thickness of the preform after being pressed with the tool T at 90ºC. 39 Fig. 3.9: Configuration of the induction plates (left) and schematic draw of the heating procedure at 20 mm (right). ... 40
Fig. 3.10: Final thickness after heating with hot air gun and cooling with tool T. ... 42
Fig. 4.1: Total function with input and output variables. ... 45
Fig. 4.2: Subsystem 1: heating ... 45
Fig. 4.3: Subsystem 2: cooling and pressing ... 46
Fig. 4.4: Subsystem 3: transport ... 46
Fig. 4.5: Subsystem 4a: cutting and stacking ... 46
Fig. 4.6: Subsystem 4b: rolling up ... 47
Fig. 4.7: Functional structure with subsystems. ... 47
Fig. 4.8: Concept 1 with infrared oven and rolling press ... 48
Fig. 4.9: Concept 2 with infrared oven and semi-continuous press ... 49
Fig. 4.10: Concept 3 with hot air and infrared ovens and rolling press... 49
Fig. 4.11: Concept 4 with hot air and infrared ovens and semi-continuous press ... 49
Fig. 4.12: Specific hot air machine for Concept 5 ... 50
Fig. 4.13: Concept 5 with hot air machine and rolling press ... 50
Fig. 4.14: Concept 6 with hot air machine and semi-continuous press ... 51
Fig. 4.15: Preference matrix ... 53
Fig. 4.16: Vulnerability analysis Concept 1 and Concept 2 ... 56
Fig. 4.17: Vulnerability analysis Concept 1 and Concept 3 ... 57
Fig. 4.18: Vulnerability analysis Concept 1 and Concept 5 ... 58
Fig. 5.1: Components of the hot air machine ... 59
Fig. 5.3: Air heating cassette ... 61
Fig. 5.4: Diagram of the needed power for different air temperatures and flow when starting from room temperature from the catalogue of Kanthal. [www17c] . 62 Fig. 5.5: Ventilator ... 62
Fig. 5.6: Plot of flow losses in circular duct. [www07] ... 63
Fig. 5.7: Dimensions and parameters ... 64
Fig. 5.8: Forces in the rollers press ... 65
Fig. 5.8: Transport process ... 66
Fig. 5.9: Distances of the pre-consolidation process in meters. ... 68
List of Tables
Tab. 2.1: Mechanic properties of fiber types. [Ege17] ... 17
Tab. 2.2: Relevant properties for different implementations. [www13a] ... 17
Tab. 2.3: Properties of various non-reinforced matrix materials. [www17a] ... 22
Tab. 3.1: Trials with manual press DEMA 1400 ... 30
Tab. 3.2: Trials heating with infrared oven and cooling with metal weight pressure. . 33
Tab. 3.3: Trials heating with oven and cooling and pressing with hand-press. ... 35
Tab. 3.4: Trials heating with oven and cooling and pressing with metal applying pressure with tools M, T and P. ... 38
Tab. 3.5: Trials heating with oven and cooling and pressing with tool T at 90ºC. ... 39
Tab. 3.6: Trials heating with oven and cooling and pressing with tool P at 90ºC. ... 39
Tab. 3.7: Trials heating with induction plates. ... 41
Tab. 4.1: Evaluation criteria ... 51
Tab. 4.2: Evaluation of the preference matrix ... 53
Tab. 4.3: Evaluation scheme with numerical values and their meanings ... 54
CF Carbon Fiber
TFP Tailored Fiber Placement
rCF recycled Carbon Fiber
RCF Reinforced Carbon Fiber
ITA Institute of Textile Technology Augsburg
Introduction and Objectives
The research of new materials is a constant of our time in all fields of engineering. One of the most important themes that the engineers investigate is the lightweight materials such as the carbon fiber which used has increased a high percentage in the last ten years. Its properties, such as high flexibility, high strength, low weight, high tempera-ture tolerance and low thermal expansion, make them very popular in the aerospace, civil engineering, military applications, motor sports or other sports. Even in jewellery when it is necessary a lightweight material with high resistance.
On the other hand carbon fiber has a really high price and the impact on the environ-ment caused by its production is more important than the impact of materials like steel and aluminium. The recycling ways of these metals are well established, while carbon fiber recycling methods have only been commercially viable for a very short time. In 2016, 18 000 tonnes of carbon fiber were produced worldwide during its manufacturing, from which only about 1 600 tonnes could be recycled. This is an enormous waste and a missed opportunity. The price of the recycled carbon fiber is almost half of virgin fi-bers and shows similar mechanical properties.
Some carbon fiber recycling methods are the chemical techniques, such as the diges-tion of resin with nitric acid; the thermal techniques, as well as pyrolysis in a controlled environment and the techniques using compression technology in which we will focus.
The Institute of Textile Technology Augsburg (ITA), investigate the processing of an automated manufacturing of rCF with a thermoplastic matrix to produce test specimens quickly and with consistent quality.
First step is the creation of RCF nonwovens with a thermoplastic matrix in an automat-ed process. Secondly a pre-consolidation process is neautomat-edautomat-ed to create a preform and finally the preform is transported with a robot to an injection moulding press (Engel in-sert 1050H 200) to produce a fiber composite work-part. A schematic vision of the pro-cess is shown in Fig. 1.1.
Fig. 1.1: Schematic vision of the overall process. The main theme of this thesis is highlighted in bold
Moreo-ver another sub-process for storing the preform is studied to be added at the end of this process.
State of the art
The fiber-reinforced composite (FRC) is a composite material that is made of three components, the discontinuous or continuous fibers, the matrix and the fine interphase region. The type of material and the process are selected according to the properties that must have the component. This work is focused only in recycling composites with carbon fibers.
In the particular case of the carbon fiber reinforced composite, it is combined a carbon fiber tissue, which provides flexibility and resistance, with a thermo-stable resin (ma-trix), which solidifies using a hardener agent and acts by bonding the fibers, protecting them and transferring the load throughout the material. The layers have a high orienta-tion which brings the high strength and stiffness of the carbon fibers. Moreover the cur-ing agent helps to transform the resin into a hard plastic. The mechanical properties of the new material are obtained from the combination of these three components.
2.1.1 Manufacturing process
Carbon fiber is a material made up of 5-10 microns diameter fibers, mainly composed of carbon atom, 90%, less than 7% nitrogen, less than 1% oxygen and less than 0.3% hydrogen.
Carbon fiber is made from another polymer, called polyacrylonitrile, through a compli-cated heating process. When the polyacrylonitrile is heated, the heat causes that the repetitive cyano units form rings. As we increase the heat, the carbon atoms get rid of their hydrogen and the rings become aromatic. This polymer constitutes a series of fused pyridine rings.
Fig. 2.1: Schematic of PAN and pitch based carbon fiber manufacturing process. [Ash13]
The structure of the carbon fiber consists of sheets of carbon atoms arranged following a regular hexagonal pattern. The layers have a high orientation which brings the high strength and stiffness of the carbon fibers.
Fig. 2.2: Structure of the carbon crystals. [Ehr06]
energy absorption. Moreover it is resistant to corrosion, moisture and to the formation of metal-carbides. Its appearance is considered elegant and its fabric texture projects luxury in its bright black colour.
The types of carbon fiber which exist nowadays can be classified according to its elas-ticity modulus:
Tab. 2.1: Mechanic properties of fiber types. [Ege17]
Mechanic properties of the C-Fiber Elasticity modulus
Ultra High Modulus (UHM) 500 Gpa
High Modulus (HM) 300 Gpa
Tensile strength/modulus minor than 1%
High Strength (HT) 3 Gpa
Tensile strength/modulus between 0.015-20
Intermediate Modulus (IM) 300 Gpa
Tensile strength/modulus around 0.01
Low Modulus Low modulus and tensile strength
According to the different implementation where it is used, some properties are more important than others, for example:
Tab. 2.2: Relevant properties for different implementations. [www13a]
Mechanical strength, resilience and density
Transports and sports goods
Dimensional stability Aerospace technology
Vibration damping, strength and resili-ence
Audio device, robotic arms, textile equip-ment…
Fatigue strength and self-lubrication Chemistry and nuclear industry
Chemist and thermic strength Electric devices
2.1.3 Recycling process
One of the main disadvantages of the carbon fiber is that due to the thermoset resins, it is a material hard to recycle. In the future with the use of thermoplastic resins this point will be easier and more viable.
Another problem is the one faced by all new materials, the lack of knowledge about the mechanical properties and lack of large-scale demonstrators which could prove the economic, technical and environmental justification for using these materials. Some justification could be, from an economic point, the use of recycled carbon fiber on its own or in conjunction with virgin carbon fibers in the industry can reduce the cost of light weighting and then increase the use of carbon fiber in much more applications. From an environmental point, is more a question of social responsibility and even in some countries a legislative requirement.
Different methods of recycling carbon fiber have been developed. They can be classi-fied in three main types of composite recycling: mechanical, thermal and chemical methods.
These processes are usually one, or more, size reduction methods applied to compo-site scrap. The large scrap pieces are size reduced by slow speed crushing, typically using a crushing mill or a large granulator. A secondary size reduction step takes place using a hammer or high-speed mills. After this, the fine particles are sorted by cyclones or sieves into fiber-rich and polymer-rich fractions. The sizes of the recycle carbon fiber are between 10 mm and 50 µm. Mechanical carbon fiber recycling has not yet been realized on an industrial scale. [Mel16]
It is the object of extensive research and can has potential for industrial application. These processes employ chemical compounds, catalysts or solvents that are used to break the chemical bonds in the polymer matrix and make the fibers free of plastic. The fibers are clean and of good quality, some studies showed tensile strength of 97% compared to virgin fibers. However, the process took 30 minutes because the reaction time is not quick and the surface of the fibers is often contaminated. If these fibers are worked into plastics, such impurity impairs adhesion of the fibers to the plastic. In addi-tion, the solvents used are often ecologically damaging. Most research into chemical recycling methods is aimed at supercritical fluids. [Mel16]
It includes pyrolysis and fluidised bed processes. These methods have a greater likeli-hood to achieve closed loop recycling, which entails recovering individual fibers, but also harnessing the reaction energy in some useful way.
oxygen, often nitrogen. Without oxygen, combustible material breaks down into lower molecular weight components and leaves char on the surface of the composite. There is a pyrolysis stage of resin degradation in air, but by removing oxygen, the degrada-tion can only reach a certain stage. The hydrocarbon products can be used as fuels to add heat to the process, since the reaction is exothermic. However since pyrolysis pro-cesses by themselves leave char on the surface of the composite, individual fibers cannot be liberated by a single process step, therefore an oxidation step is required to remove the char and recover the fibers.
The fluidised bed recycling consists of a bed of silica sand with average particle diame-ter minor than 1 mm. The sand is fluidised by a stream of hot air passing through a distributor plate, at a superficial speed in excess of 0.4 m/s at a temperature typically above 500ºC. The resin burns off the composite and the char degrades, when sufficient char has degraded, individual fibers break off and are elutriated/filtrated along with the gases released from the resin. Following elutriation/filtration, the fibers are separated from the gas stream by a cyclone separator and deposited into a collection bin. The gas stream enters a secondary high temperature combustion process in order to oxi-dize them. [Mel16]
Fig. 2.3: Graphic of composite demand and waste in kilotons per year. [Mel16]
Composite materials are made of fibers as reinforcement and of different materials that work as a matrix. The matrix surrounds fibers and protects against chemical and envi-ronmental attacks. For fibers that resist strong loads the matrix must have less modu-lus and much more stretching than the reinforcement. The choice of the matrix is based on the chemical, thermal environmental, cost, performance and manufacturing re-quirements. The matrix establishes the operating temperature of the composite, as well as the manufacturing parameters to be used in their processing.
There are different materials used as matrix:
- Polymer matrix
- Thermosets curing
- Polyester resins
- Vinyl resins
- Phenolic and carbon matrix applied to a mould or a material for curing. The curing process takes place as bonds form and heat is present. These bonds change the basic nature of the material chang-ing the once liquid resin into a solid material. Once cured the thermoset cannot longer be melted. Thermoset polymers have sites along the polymer chain that can be acti-vated to become reactive. These sites react in a way that chemical bonds are formed between adjacent polymer molecules. This crosslinking formation is what cures the material and hardens it. When bonds form they restrict the motion of the polymer mole-cules to an increasingly greater amount. There are several disadvantages to thermo-sets, including: processing time, vapours, limited shelf life, inability to reprocess and a poor toughness.
The types of matrix material are:
Polymer: in this type of matrix, monomers are linked together into short chains called
oligomers that are then bonded together leading to a polymer molecule. Many varia-tions of polymeric matrix exist for predetermined properties. Some common thermosets include polyester, vinyl ester, epoxy, phenolic, cyano-acrylate and polyamide.
Polyester resin: is the cheapest and most widely used matrix in conjunction with
Epoxies: are the second most common thermosetting polymeric matrix materials. They
have excellent adhesion, shear strength, fatigue resistance, strength and stiffness when compared to polyesters. The increased mechanical properties of epoxy are di-rectly related to an increase in cost.
Polyamide: is the material used in the ITA. The procedure resembles a process
Thermoplastic composite materials are becoming more popular and have increased properties making them used in an increasing number of applications. Structural ther-moplastics in particular have become a prevalent alternative to thermosets due to their enhanced mechanical properties, differences in processing capabilities, and manufac-turing benefits.
Thermoplastic resins are solid at room temperature and are processed significantly differently than liquid thermoset resins. With appropriate pressures parts are fabricated with low void content and can be recycled. Thermoplastic composite have the added benefit of being able to be stored at ambient temperatures, so there is no need of re-frigeration. Thermoplastics are heated and softened for application into a mould and then allowed to cool into the new shape. The great advantage of thermoplastics is that the shape is not an irreversible process. Within a certain temperature range thermo-plastics may be melted again or heated and deformed again without that leads to sharp fluctuations in material properties. The ability to reform and reshape parts is beneficial in many applications and for recycling without damaging the fibers by high tempera-tures. However care needs to be taken to make sure temperatures are adequate for the design. [Ege17]
Tab. 2.3: Properties of various non-reinforced matrix materials. [www17a]
Property Polyesters Epoxies
number of materials from the definition, including paper, products which are woven, knitted, tufted or stitchbonded (incorporating binding yarns or filaments), or felted by wet-milling, whether or not additionally needled.
2.3.1 Manufacturing process
Nonwovens can be subdivided based on the fiber layer into three groups: wetlaid, spunbond and drylaid nonwoven.
For wetlaids mainly short cut fibers, in a range of 5 mm to 30 mm are used. These are first dissolved in a strong dilution in water, similar to the paper production, and then placed over a sieve. A thermal or chemical solidification of the fibers then takes place. This kind of fleece is very dense, has isotropic properties due to the random fiber tray and thus achieved good strength values. In contrast, continuous fibers are used in the spunbond webs, which are spun only during the nonwoven production. For this pur-pose, the granules are fed into the spinning nozzles via an extruder. After that, a tar-geted deposition of the fibers can take place, whereby the properties can be defined more precisely. The solidification can be carried out here both thermally, chemically and mechanically, depending on the weight. Here, too, as with the wetlaids high strength and a high density are obtained. [AVK14]
The drylaid process used in the nonwoven compact-installation of the ITA is explained in next sub-chapter.
2.3.2 Preparation to the Dilo compact fabric conditioning
On the ITA available Dilo KO1.34290.16 ITA compact system (Dilo) the webs get dry by dry laying process of staple fibers, that is fibers of finite length made from rCF. In Fig. 2.4 the Dilo machine is shown.
Fig. 2.4: Side view of the Dilo machine used by the ITA. [Mar17]
chamber. After the feeding, the fibers are combed on the morel and transferred to the carding machine. There the fiber web is produced over the main drum and attached to their workers-turner pairs. In the successive laying, the web can then be settled to the thickness required for the desired fiber weight. For this purpose, several nonwoven layers are superposed, in different orientations, and weights up to 200 g/m2 and more can be achieved. The orientation chosen for this is just as important as the fiber weight for the strength properties of the finished nonwoven.
To solidify, the mechanical version of the needling is used in the Dilo machine. Through a needle board, the fibers are looped from above and below each other. Depending on the strength of this entangled, the nonwovens are subsequently either very strong and thus only slightly pliability, or have a lower density and thus a higher pliable capacity. In contrast to chemical hardening, no additional binders are required in this variant. Thermal consolidation is limited mainly to polymer fibers. [Ege17]
Instruments of development methodology
Fig. 2.5: General procedure for developing and designing. [PBF07]
From the requirement list, the elementary requirements are filtered and the functional structure is defined. The purpose of the functional structure is to solve problems that are simple and variant-solvable. For this purpose, the overall function is subdivided into sub-functions, as shown in Fig. 2.6.
Fig. 2.6: Overall function divided into sub-functions. [Fel13c]
The sub-functions are further decomposed and returned to functions. An elementary function is by definition the description of the primary function of a technical structure. Primary functions are functions which convert, for example, energy, material and / or signals. The return to elementary functions is helpful since various functions can be used for these functions. The functional structure must be neutralized so that solutions are not excluded at the beginning of the design process. [PBF07, Kol98]
Evaluation of concepts
evaluation and 4 stands for an ideal solution based on the evaluation criterion. The total value of each solution concept is the sum of the product of weighting and point allocation of the respective evaluation criterion. The highest overall value identifies the favoured concept, [PBF07, Rin14].
Vulnerability analysis reveals possible deficits in the design. Often it is possible to elim-inate these deficits in further development. A graphical representation is used here in order to be able to easily identify weak points, in this work the so-called value profile is used, which is based on a bar chart. Fig. 2.7 shows an example of such a value profile. Each evaluation criterion is represented by a bar. The length of the bar corresponds to the selected value of the concept in relation to the criterion. The height of the bar re-flects the weighting of the assessment criteria. The resultant area corresponds to the weighted partial values. This type of graphical representation makes it easy to deter-mine which criterion has to be improved in order to increase the overall value. A bal-anced value profile is aimed at [PBF07]. With the vulnerability analysis, the final selec-tion is made, of which of the concepts is further developed. [Rin14]
It has been done four types of trials: heating up with the manual press, heating up with infrared oven, heating up with induction plates and heating up with hot air. For each of these trials it has been selected a way of cooling down and pressing. The possible way have been: cooling with a metal weight, with a hand-press and with three cooling tools that have a small pressure area.
The aim of the present work is to figure out new effective process to do the pre-consolidation of the hybrid textile for the production of parts. This includes doing it fast-er and look for a continuous way of doing it in the future. The preform process is nowa-days a manual and long process that needs labour and it is only available for discrete manufacturing. For this purpose it has been tried three other sources of heating like infrareds (infrared oven), induction (induction plates) or hot air (hot air gun). The results obtained with the hot air have been satisfactory for pre-heating in the pre-consolidation process because of the low time that it took to heat the surface in the trials. However to heat all the preform, not only the surface, the hot air seems the best options to improve the process and to reach the objective of a continuous process. On the other hand it has been shown that heating by induction is a long and inefficient way to heat the pre-form.
Introduction and objectives
The consolidation process aims at transforming the nonwoven material into a pre-form that can be used to create the web based thermoplastic composite. To reach this objective the hybrid textile has to be heated till its melting point and then quickly cooled down and pressed before it gets stiff again.
Trials heating with the DEMA Hand-press TP1400
Nonwoven textile 40% rCF / 60% polyamide
DEMA Hand-press TP1400
Airtech MR1 separation film
Metal weight of 25 kg
First trials have been made heating with the DEMA Hand-press TP1400 and then cool-ing down and presscool-ing by contact pressure with a metal weight of 25 kg with a surface temperature of 22ºC during all the trials. The force applied has been:
g m/s (3.1)
in an area of:
A m m m (3.2)
To prevent the sticking of the layers with the Hand-press and the cooling metal, the layers were covered with the Airtech MR1 separation film.
Trials heating up with infrared oven
Infrared oven (Fig. 3.1).
Fig. 3.1: Infrared oven. [EnM16]
Nonwoven textile 40% rCF / 60% polyamide
Pressing tools used:
Metal weight of 25 kg
DEMA Hand-press TP1400
Cooling and pressing metal tools M, T and P with different contact areas: 2.25 cm2 (M), 7 cm2 (T) and 10 cm2 (P).
In these trials the heating source selected has been an infrared oven. The layer is put on the sliding tray and then introduce into the oven when this one is already at the de-sire temperature. On the first trials it has been shown that when the hybrid textile was heated in the infrared oven it started to blend so the solution has been to put a metal grid upper the material to do not permit the blending. This problem solved, the trials have started again with a temperature in the oven of 275ºC, higher than the melting temperature of 246ºC, testing a time between 60 to 10 seconds to try to find the best relation time/temperature to have a good preform in the least time possible.
been to pressure with a metal tool with a pressure area between 2 and 10 cm2. Each type of pressing is explained in more details in the next sub-chapters.
3.4.1 Cooling and pressing with metal weight applying contact pressureFor this trial a force of 245 N has been applied with a 25 kg metal weight, with a sur-face temperature of 22ºC during all the trials, to cool and press the preform like in the trials of chapter 1.2.
The first trials have been made heating during 60, 30, 25, 20 and 10 seconds at the temperature of 275ºC to then can conclude which was the minimum time enough to make a preform similar to the ones used before. The pressure has been applied 10 seconds after the heating and during 60 seconds. These times have not changed. Trials have been made with one layer, with two layers already heated and pressed and with four (2 layers heated and pressed + 2 other ones). A layer before working on it and another after are shown in Fig. 3.2.
The trial parameters and some notes about the results are summarized in Tab. 3.2.
Tab. 3.2: Trials heating with infrared oven and cooling with metal weight pressure.
Fig. 3.3: Two layers heated together in the oven 20 seconds (left) and 30 seconds (right).
3.4.2 Cooling and pressing with metal applying pressure with the DEMA
Tab. 3.3: Trials heating with oven and cooling and pressing with hand-press.
There is a difference between the temperature of the upper pressing plate (Tu) and
the lower (TL) because the Hand-press only heat up the upper one.
Fig. 3.4: Final thickness of trials P1, P2 and P3.
For the cooling side, these trials show that when the pressing tool gets heated till 70ºC the results start to be worse, the thickness begin to increase, as it can be seen in Fig. 3.5. Another remark is that from 70ºC to 90ºC of the pressing tool the results are similar so it is not worth to cool it down in this range.
Fig. 3.5: Final thickness with the hand-press at 90ºC.
3.4.3 Cooling and pressing with metal applying contact pressure in a
Fig. 3.6: Schematic draw of each way of applying pressure used.
The heating temperature in the infrared oven has been of 275ºC during 30 seconds in every trial. Two cooling and pressing tools have been used, one with a contact area of 2.25 cm2 (M) and the other with a contact area of 7 cm2 (T). The pressure applied has been firstly between 40 and 50 N and then between 60 and 90 N. The last part of the trials has been to measure with an electronic caliper the final thickness of the preform (Fig. 3.7) to appreciate the quality of each process. In Tab. 3.4 every parameter are showed.
Tab. 3.4: Trials heating with oven and cooling and pressing with metal applying
pres-Looking at Tab. 3.4, from the three ways of applying pressure, it can be said that “Hit-ting” is not a good solution; the final thickness is the highest, more than 2 mm “Sliding” could be a method to develop because the thickness obtain is nearly 1 mm in both tri-als done. The best method seems to be “Pressing” during seconds to have a preform thickness of 1 mm. However 4 seconds could also being enough because the results are very similar, less than 0.20 mm of difference between trials M2 and M3 and be-tween T2 and T3.
Fig. 3.8: Final thickness of the preform after being pressed with the tool T at 90ºC.
Tab. 3.5: Trials heating with oven and cooling and pressing with tool T at 90ºC.
Trials Layers Tcooling
Moreover a cooling and pressing trial with tool P at 90ºC has been made. Tool P has been pressed with the DEMA Hand-press TP1400 settled at 90ºC also.
Tab. 3.6: Trials heating with oven and cooling and pressing with tool P at 90ºC.
Trials heating up with induction plates
IFF induction plates EW200NTW
Nonwoven textile 40% rCF / 60% polyamide
Piece of metal
Airtech MR1 separation film
Next trials have been done with two IFF induction plates that use the robot to heat the preform after the pre-consolidation process. The configuration of the induction plates can be seen in Fig. 3.9.
Fig. 3.9: Configuration of the induction plates (left) and schematic draw of the heat-ing procedure at 20 mm (right).
Tab. 3.7: Trials heating with induction plates.
T0 is the initial temperature of the hybrid textile and Tf is the temperature after
heating the preform.
After these trials it seems that the induction plates of the robot, currently specified to heat steal do not work efficiently with the preform. The induction plates heat quickly the metal but would need more than an hour to heat the hybrid textile. A solution could be to try the heating with other induction plates that are not so specific to heat steal or to vary the frequency parameter.
Trials heating with hot air
Bosch hot air gun PHG 500-2
Nonwoven textile 40% rCF / 60% polyamide
Cooling tool T
Fig. 3.10: Final thickness after heating with hot air gun and cooling with tool T.
In this chapter are presented theoretical instruments of development methodology, in chapter 4.1 the concept requirements are listed. Secondly in section 4.2 the functional structure is settled and divided into sub-functions. Next step is to define each of the concepts in chapter 4.3. In section 4.4 a review of the concepts is carried out and in chapter 4.5 a vulnerability assessment is created to select a final concept for further definition of it.
The list of requirements includes main features that provide information to find the rele-vant requirements. They are distinguished in two types: the mandatory ones, listed with (P), which describes the primary function of the system. And the requests (S) that con-tain information on requirements to be considered if possible. The requirements are listed as sub-items of each main feature and then summarized in the request list.
The heating tools designed have to be able to heat at least till 300ºC to ensure that they can reach easily the melting temperature of the nonwoven material, 246ºC. More-over they must heat up continuously and in a uniform way to permit the heating of all the part. The preform has not to be heated only in the surface but also inside, if not the pre-consolidation process will not be achieved satisfactorily.
It is required that enough contact pressure (min a force between 60 and 150 N) is ap-plied in the perpendicular direction of the preform after it has reached the melting tem-perature. Also the time passed after the heating process must be lower than 12 seconds to do not permit that the textile turns solid again.
The module shall not require exceptional demands on the power supply and the con-nections of the existing infrastructure of the ITA.
The heating sources must be closed and with all the hot cables cover by an isolating material to prevent possible accidents of the workers. Moreover it has to be at least one fire extinguisher in each heating machine.
The production time must be as low as the costs permit it. Tools used should not have an excessive price. Furthermore the storage of the final preform must not take so much place. chine and the injection moulding press are not in the same place.
Ideally for any customer is that the unit designed is free of maintenance. This is not usually possible; nevertheless the hypothetical reparations should be done easy and quickly. This means that the main module can be disassembled and that the parts are easy to replace.
The separation of the different materials which are not recycled in the same way have to be possible to accomplish the law.
4.2.1 Building the overall function
The purpose of the process is to make the pre-consolidation part of the web. This in-cludes a heating process of the hybrid textile followed by a cooling and pressing pro-cess and if possible a rolling or cutting and stacking propro-cess. Moreover the transport of the preform is also needed. In Fig. 4.1 it is shown the total function with input and out-put variables.
Fig. 4.1: Total function with input and output variables.
The preform is took from the nonwoven machine and then transported in a ribbon dur-ing the pre-consolidation process. First the preform is heated at least till the meltdur-ing temperature between 245ºC and 260ºC. Secondly the web is pressed and cooled down and then rolled or cut and stacked.
4.2.2 Dividing the overall function into sub-functions
The next step is to divide the overall function into sub-functions. These sub-functions are considered as individual subsystems for a better overview. The subsystems con-sidered are:
Heating (subsystem 1)
The first subsystem processes the heating of the preform that have to reach the melt-ing temperature.
Fig. 4.2: Subsystem 1: heating
Cooling and pressing (subsystem 2)
Fig. 4.3: Subsystem 2: cooling and pressing
Transport (subsystem 3)
The preform has to move from one operation to the next, this can be done automatical-ly or manualautomatical-ly. In the first case it can also be continuous (better if the pre-consolidation form structure is built after the nonwoven machine) or discontinuous if the heating pro-cess needs to be longer in time but not in length.
Fig. 4.4: Subsystem 3: transport
Cutting and stacking (subsystem 4a)
One option after cooling down the preform is to cut it and then stack it to have the pre-form already prepared to use in the machine which create the web.
Rolling up (subsystem 4b)
The second option is to roll up the preform to permit an easy storage and future trans-portation to the cutting tool.
Fig. 4.6: Subsystem 4b: rolling up
4.2.3 Complete functional structure
In Fig. 4.7 the complete functional structure is summarized with all the subsystems.
Definition of the concepts
Six different concepts are proposed with subsystems 1 and 2 defined in each sub-chapter. However subsystem 3 is the same for all of them, the preform is transported during the process by a continuous conveyer belt. Finally subsystem 4 can be indis-tinctly chosen between 4a and 4b.
A continuous belt is selected as subsystem 3 for the transport of the preform during the process in all the concepts. The main reason that this continuous process has been chosen instead of the use of a robot it is because it permits to assemble the pre-consolidation process at the end of the nonwoven machine that uses a continuous pro-cess too. Moreover a robot will increase the investment costs and the maintenance without improving the quality of the final preform. Another option considered has been to use the robot that put the preform into the injection moulding press, but there is not enough space to place a pressing and cooling tool and the press used for producing the final parts is not adaptable to the pre-consolidation process.
4.3.1 Concept 1
The subsystem 1, which processes the heating of the preform, is implemented by an infrared oven. For the next subsystem it has been selected a rolling press that includes two parallel rollers with the same dimensions.
Fig. 4.8: Concept 1 with infrared oven and rolling press
4.3.2 Concept 2
Fig. 4.9: Concept 2 with infrared oven and semi-continuous press
4.3.3 Concept 3
This concept has a subsystem 1 composed of a hot air oven and an infrared oven. The subsystem 2 is the same that the one from Concept 1 with the rolling press.
Fig. 4.10: Concept 3 with hot air and infrared ovens and rolling press
4.3.4 Concept 4
The subsystem 1 of concept 4 is the same as concept 3, infrared oven after a hot air oven. Subsystem 2 is a semi-continuous press.
4.3.5 Concept 5
Concept 5 uses a specific hot air machine that recirculates the air and permit to pass it inside the textile so that it heats properly. The subsystem 2 is a rolling press like the one used in concept 1 and 3.
Fig. 4.12: Specific hot air machine for Concept 5
4.3.6 Concept 6
For concept 6 the same subsystem 1 as in concept 7 is used. The subsystem 2 is a semi-continuous press like in concept 2 and 4.
Fig. 4.14: Concept 6 with hot air machine and semi-continuous press
Assessment of Concepts
To select the solution concept we used the evaluation criteria presented in Tab. 4.1: Evaluation criteria.
Tab. 4.1: Evaluation criteria
High production speed
2. INVESTMENT COSTS
3. RUNNING COSTS
Durability of the designed components
Central control unit
Visual control needed
Quick stop option or safe mode
Good isolation of burning or electrifying cables
7. CORRECT HEATING
Melting point achieved in all the preform
Part not burned
Uniform temperature distribution
8. COOLING AND PRESSING
Uniform distribution of the force in all the surface
Minimum pressure between 60 and 150 Newton
Controlled temperature of the pressing tool
Low waste of energy
Recycling of the materials that are used during the process and have to be replaced by new ones
Fig. 4.15: Preference matrix
The frequency of the corresponding numbers of an evaluation criterion in the prefer-ence matrix reflects the importance of the criterion. In order to normalize this, the fre-quency is in Tab. 4.2 divided by the number of all combinations (45) and there is a normalized weighting factor for each evaluation criterion.
Tab. 4.2: Evaluation of the preference matrix
1 2 3 4 5 6 7 8 9 Σ
Frequency 6 8 5 7 3 2 6 5 3 45
The table shows that the evaluation criterion of the Investment costs (2), with eight nominations, has the highest importance of all criteria. Furthermore, the maintenance (4), with seven nominations has a great importance too. Less important in the following evaluation is the safety (6) followed by the Control (5) and the Efficiency (9).
After these results, it is clear that the focus is on the economic aspects which are the most important for the customers. However the good functionality of the process (speed, temperature, pressure) seems also important and plays a subordinate role. The safety and control do not be so important because the present design is a proto-type and the focus is on reaching a good quality product taking care of the costs.
In the following rating scheme (Tab. 4.3), the numerical values are fixed and each of them associated with one meaning. The scale used is from (“unsatisfactory”) to (“ideal”) Often it is not possible to assign a value to a qualitative evaluation criterion For this reason, the concepts are compared between each other and not with an ideal solution. The comparison with an ideal solution would be an absolute comparison. The scale of importance when comparing thus changes to "well below average" to "well above average".
Tab. 4.3: Evaluation scheme with numerical values and their meanings
Points Importance Significance when
0 Unsatisfactory Well below average
1 Just about acceptable Below average
2 Sufficient On average
3 Good Above average
4 Ideal Well above average
Tab. 4.4: Concept comparison analysis
N. = number of criterion; Wt.fct. = Weighting factor; V. = value of the criterion; Vt. = total value; Wt Wt fct The explanation of each value is shown in A.1.
In Fig. 4.16 the concept 1 is compared with the Concept 2 that has a different pressing tool. From the figure, it appears that the Concept 1 is balanced overall. It has a high rating in each criterion and every rating is equal or higher than the one from Concept 2. In concept 2 the weaknesses are the safety (V6) and the cooling and pressing (V8). The more important is the cooling and pressing because it affect directly in the produc-tion of the preform. The safety has not a bad score (2, sufficient) and can be improved with some extra protection of the semi-continuous press.
Fig. 4.16: Vulnerability analysis Concept 1 and Concept 2
Fig. 4.17: Vulnerability analysis Concept 1 and Concept 3
Fig. 4.18: Vulnerability analysis Concept 1 and Concept 5
Development of the concept
This chapter describes the steps of the design for the concept 5. The dimensioning and the configuration of each of its individual components are explained in the next sec-tions. The hot air machine for the heating process is explained in chapter 5.1, the roll-ing press for the coolroll-ing and pressroll-ing process is defined in chapter 5.2, the rollroll-ing pro-cess to get the material in rolls is described in chapter 5.3 and finally, in chapter 5.4, the conveyors for the transport process is defined.
The heating process
A hot air machine is used for the heating process. The components of this machine are an air recirculation system with a filter, an air heating cassette to heat the air up and a ventilator. In Fig. 5.1 every part of is shown.
Air recirculation with filter
The hot air after heating the hybrid textile has to be cleaned of possible particles. For this purpose a filter resistant to high temperatures is needed. The filter is not regener-ated because the carbon fibers need to be heregener-ated till 2 000ºC to get burned and this temperature is very far from the 300ºC settled in the process. In Fig. 5.2 the recircula-tion system with the filter is shown.
Fig. 5.2: Air recirculation with filter
Air heating cassette
Fig. 5.3: Air heating cassette
The power needed to heat the air till 300ºC can be deduced from Fig. 5.4 depending on the air flow wanted. In the trials of chapter 3.5 with the hot gun the flow has been be-tween 24 m3/h and 30 m3/h through an area of:
A m m (5.1) So the speed of the flow has been:
A v v m /h
The flow can expected to be between 20 000 and 25 000 m/h.
For the area wanted of
A m m (5.3)
the flow should be
A v m m/h m /h (5.4)
The flow that has been taken into account is between 4 000 and 5 000 m3/h.
And the power has been obtained from the curves of Fig. 5.4. With the air at 200ºC the power needed to heat a flow of 1 400 m3/h is 100 kW so the flow of the process has been obtained interpolating the numbers between 200 and 400ºC.
Fig. 5.4: Diagram of the needed power for different air temperatures and flow when starting from room temperature from the catalogue of Kanthal. [www17c]
To generate the necessary air flow that penetrate the preform and heat it inside, a tubular and axial ventilator is needed. The flow needed is the one calculated before, between 4 000 and 5 000 m3/h. The ventilator is shown in Fig. 5.5.
Fig. 5.5: Ventilator
To move this flow the power supplied must be:
W hp g
m / Pa m W
The flow losses (hp) value has been taken from Fig. 5.6.
Fig. 5.6: Plot of flow losses in circular duct. [www07]
The Cooling and pressing process
In Concept 5 the way of cooling and pressing is using a rolling press. The parameters of the press are the previous thickness (h0), the final thickness (hf), the lineal speed of
the rollers (Vr), the projected length of the contact arc (Lp) and the contact angle (α)
Fig. 5.7: Dimensions and parameters
The relationship between the diameter of the rollers, the contact angle and the absolute reduction magnitude is expressed by the formula:
h hf ( cos α) (5.6) so the absolute reduction magnitude rises with the increasing of the rollers diameter.
And the maximum reduction possible is defined by the formula:
h max (5.7)
tan α (5.8)
Fig. 5.8: Forces in the rollers press
Data of the pre-consolidation process here designed
Initial thickness of the hybrid textile produces by the nonwoven machine: ho = 10 mm, the same as the one used in the preliminary trials
Final thickness needed: hf = 1 mm, the same as the better obtained in the preliminary trials in sub-chapter 3.4.3.
Radius of the rollers: R = 0.15 m
h h hf mm mm mm (5.9) Projected length of the contact arc:
p √ h √ m m m (5.10)
h hf ( cos α)
α arcos ( (h hf)) arcos ( ( mm mm
So the contact angle has to be 14º at least.
The force of the rollers is calculated from the preliminary trials with the reduced area pressing tool T (sub-chapter 3.4.3). The pressure of the trial is deduced:
The contact area of the rollers is (wi = width of the material):
A wi m m m (5.13)
So the force of the rollers is:
P A Pa m (5.14)
The force of the rollers can expected to be between 35 000 and 40 000 N.
Lineal speed of the rollers: from the preliminary trials of sub-chapter 3.4.3, before men-tioned, the time of pressing (tP) needs to be between 3 and 5 seconds so:
The lineal speed has to be between 0.008 and 0.02 m/s.
Angular speed of the rollers:
w r m/s
W w p w m rad/s W (5.17)
The transport process
The transport of the material is done by a conveyor which is put into operation through the motor system; the movement to the belt is imparted by the driving drum, through the transmission system. The belt is the traction member of the conveyor and at the same time the material transport. The preform is automatically deposited therein by the nonwoven machine which supplies the material constantly to the conveyor. At the end the material is rolled. Fig. 5.8 shows the transport system.
The speed of the conveyor is defined by the speed needed in the infrared oven and in the rollers. It is adjustable increasing or decreasing manually the power that arrives to the driving drums and it is constant.
The power needed can expected to be between 100 and 400 W as it is said in the Ax-mann catalogue [www17d].
The rolling up process
After cooling down the material, it is rolled up in big rolls to facilitate the transport. The preform can be bended till 20 degrees, so the rolls have to have a diameter higher than 15 centimeters. The diameter chosen for the calculations is 20 centimeters.
The time to roll 1 meter can expected to be between 20 and 25 seconds.
Total production and energy consumption
The production time of 1 meter of preform is the same time as the rolling up time of 1 meter (between 20 and 25 seconds). So the total production (PrT) is:
Pr m s
The total production can expected to be between 140 and 180 m/h of preform.
If the speed of the process (vT) needs to be increased, then the lineal speed of the
roll-ers (Vr) also, to do that it is necessary to increase the angular speed of the rollroll-ers (w) or the radius of the rollers (R).
The energy consumption is:
H P r W W W W W
The total energy consumption of the pre-consolidation process can expected to be be-tween 1 200 and 1 500 W.
The length of the pre-consolidation process is shown in Fig. 5.9.
Summary and Outlook
The ITA developed a process to create an rCF part from RCF nonwovens with a ther-moplastic matrix. This process is divided in three steps: the nonwoven process, the pre-consolidation process and the moulding and injection process. (At the moment the three steps are divided in different places but the pre-consolidation process can be adapted at the end of the nonwoven machine.)
The pre-consolidation process of the hybrid textile is needed to have a preform worka-ble for the injection moulding press. To achieve a good quality of the preform, the tex-tile has to be heated till the melting point and then quickly cooled and pressed. This process needs to be updated to another more efficiently and faster that allows a more automated overall process.
To develop the new pre-consolidation process some preliminary trials about the way of heating and cooling and pressing have been performed and a theoretical design has been done. For the design, first of all the list of requirements has been defined and then the functional structure of the pre-consolidation process. Using the theoretical knowledge and the preliminary trials six concepts have been defined and evaluated depending on some concrete criteria. Then the most interesting have been compared by value profiles.
The chosen concept heats the textile with a hot air machine that heats the preform into its core, then a rolling press is used to do the pressing and cooling process and finally a roll helps to storage the preform obtained. During the process the material is guided by an automatic conveyer belt. In Fig. 6.1 the hot air machine composed by a ventila-tor, an air heating cassette and an air recirculation system with filter is shown.
Fig. 6.1: Heating system of the developed concept
preliminary trials of chapter 3. The air flow and the heating time of the hot air machine are calculated after the trials with the hot air gun and the dimension, the force and the speed of the rollers are based on the trials with the reduced area pressing tool. With the developed concept, the pre-consolidation process is turned into a continuous pro-cess and achieves a production between 140 and 180 m/h of preform.
[Ash13] Ashraful Himel
Formation of Carbon Fiber and Application. 1st Ed Bangladesh: Southeast University, 2013
[AVK14] AVK-Industry Asociation Reinforced Plastics
Manual Fiber Composites/Composites, Basic-Processing. 4th Edition Wiesbaden: Springer Vieweg, 2014
[Cha12] Chawla K.
Composite Materials. 3rd Ed Alabama: Springer, 2012
[Ege17] Eger E-M.
Process development for the production of test specimens by pressing of carbon-fiber-nonwovens with a thermoplastic matrix
Augsburg, University of augsburg
Institute of Textile Technology Augsburg, 2017
[Ehr06] Ehrenstein, G.W.
Fiber composite plastics, materials, processing, properties. 2nd Edition Munich: Carl Hanser Verlag, 2006
[Ehr11] Ehrenstein, G.W.
Polymeric Materials: Structure, Properties, Applications. 3rd Ed. Munich: Carl Hanser Verlag, 2011
[EK14] Emmerich R., Kuppinger J.
Operator Manual Machine IN 1050H/200
Composite Materials (2014), Vehicle Engineering, P. 62-65
[EnM16] Engel Austria GmbH (Hrsg.) Recovering Carbon Fibers
Schwertberg: Engel Austria GmbH, 2016, [Firmenschrift]
[Fel13c] Feldhusen, J.
Vorlesungsunterlagen: Konstruktionslehre I – Vorlesung 2, Konzeptentwicklung I
https://www.ikt.rwth-aachen.de/fileadmin/downloads/KL_I/V02_-_Konzept_1.pdf [Stand 12.01.2014]
[Fel13d] Feldhusen, J.
Vorlesungsunterlagen: Konstruktionslehre I – Vorlesung 13, Bewerten von Lösungen
[Kol98] Koller R .
Principle solutions for technical products construction. 2nd Ed Berlin: Springer, 1998
[Mar17] Marin, P.
Erarbeiten von Anlagenparametern zur Erzeugung von Vliesstoffen unterschiedlicher Orientierung und deren Vergleich, Augsburg, Universität Augsburg, Institut für Textiltechnik Augsburg gGmbH, Bachelorarbeit, 2017
[Mel16] Melendi-Espina S.
Recycling of carbon fibre composites Penn State University
Carbon 2016, Penn, 2016
[Mor05] Morgan P.
Carbon Fibers and Their Composites. Edition with number New York: Taylor & Francis, 2005
[Pag00] Page I.
Polyamides as Engineering Thermoplastic Materials. United Kingdom: Rapra, 2000
[PBF07] Pahl G., Beitz W., Feldhusen J., Grote K-H.
Pahl / Beitz Engineering Design. Basics of successful product development methods and applications. 7th Ed
Berlin: Springer, 2007
[PPS16] Pelin C-E., Pelin G., Stefan A. and more
Mechanical properties of polyamide/carbon-fiber-fabric composites Materials and Technology 50 (2016), P. 723
[Rin14] Rinno M-P.L.
Construction of an adaptive pressing unit for homogenizing unfixed multiax-ial
Aachen, University of Aachen
Institute of Textile Technology Aachen, 2014
[Ste16] Stevenson A.
Recycling carbon fibre: state of the art and future developments Aachen, Dresden, Denkendorf Universitys
International textile conference, Dresden, 2016
[WR14] Worrell E., Reuter M.
Handbook of Recycling: State-of-the-art for Practitioners, Analysts, and Scientists. 2nd Ed
London: Elsevier, 2014
[www13] https://myprofetecnologia.wordpress.com/2013/02/10/los-nuevos-materiales/, 10.02.2013
[www17a] http://www.commonfibers.com/what-is-carbon-fiber, 2017
[www17b] https://www.edana.org/discover-nonwovens/how-they%27re-made/formation, 2017
[www17c] http://www.kanthal.com/en/products/furnace-products-and-heating-systems/air-heating-cassettes/, 2017
A.1: Explanation of values for each concept of Tab. 4.4.
Value explanation mized and the security rules are accomplished. Moreo-ver the way of heating with the infrared oven has been tested in the trials of chapter 3.2 with good results.
Concept 2: infrared
This concept has similar criteria values as concept 1. However the cooling and pressing value is lower (2, sufficient) because the press used is a semi-continuous one which can damage the textile with its movement by creating wrinkles or can leave some surface not pressed because of an offset between the press and the textile. The safety is also worse because the semi-continuous press can damage something or hurt some-one with its movement.
Concept 3: hot air
and infrared oven and rolling press
In this concept there is two ways of heating so the cor-rect heating value is the maximum (4, ideal). On the other hand the investment and running costs values decreases because the hot air oven is an additional expense that is not in Concept 1 and 2.
Concept 4: hot air
and infrared oven and
The values for Concept 4 are similar as the values from Concept 3 because it has the same way of heating. The safety and cooling and pressing values are lower be-cause of the semi-continuous press (same reason as in Concept 2).
Concept 5: hot air
machine and rolling
aparezca aquí. 75
Concept 6: hot air
machine and semi-continuous press
Statement of academic honesty
I hereby declare to the best of my knowledge that this thesis contains no material pre-viously published or written by any other person. The work submitted in this thesis is the product of my own original research, except where I have duly acknowledged the work of others.